Title Preparation of chemically modified RNA origami
Preparation of chemically modified RNA origami
Endo, Masayuki; Takeuchi, Yosuke; Emura, Tomoko; Hidaka,
Kumi; Sugiyama, Hiroshi
Chemistry - A European Journal (2014), 20(47): 15330-15333
This is the peer reviewed version of the following article:
Endo, M., Takeuchi, Y., Emura, T., Hidaka, K. and Sugiyama,
H. (2014), Preparation of Chemically Modified RNA Origami
Nanostructures. Chem. Eur. J., 20: 15330‒15333, which has
been published in final form at
http://dx.doi.org/10.1002/chem.201404084. This article may be
used for non-commercial purposes in accordance with Wiley
Terms and Conditions for Self-Archiving.; 許諾条件により本
Preparation of Chemically Modified RNA Origami Nanostructures
Masayuki Endo,*[a][c] Yosuke Takeuchi,[b] Tomoko Emura,[b] Kumi Hidaka,[a] and Hiroshi Sugiyama*[a][b][c]
Abstract: RNA molecules potentially have structural diversity and
functionalities, and it should be required to organize the structures
and functions in a designed fashion. We developed the method to
design and prepare RNA nanostructures by employing DNA origami
strategy. RNA transcripts were used as a single-stranded RNA
scaffold and staple RNA strands for the formation of RNA
nanostructures. After the annealing of the mixtures, we obtained 7helix bundled RNA tile and 6-helix bundled RNA tube structures as
predesigned ones. These nanostructures were easily functionalized
by introduction the chemical modification to the RNA transcripts. The
DNA origami method can be extended and utilized to construct RNA
RNA nanotechnology is an emerging research field that has
potential for applications in the imaging, diagnostics, and
regulation of cell functions.[1–3] RNA molecules have structural
diversity, which provides unique functions, such as catalysis and
binding to specific molecules. Functional RNAs have been
explored by in vitro selection to create artificially ribozymes and
aptamers. Riboswitches and short interfering RNAs (siRNAs)
are now used to regulate gene expression. For the
construction of RNA nanostructures, small structural motifs have
been used to build up 2D and 3D structures with
functionalities.[6–9] Although RNA molecules have fascinating
functions, the available structural motifs of short RNAs are
limited; thus, it is still challenging to design RNA nanostructures
artificially. To expand the variations of the RNA structures, we
designed and constructed RNA nanostructures in a similar
fashion to that used in DNA origami design.[10,11] Recently,
RNA/DNA hybrid nanostructures were created to expand their
structures, with synergistic effects.[12–14] Furthermore, RNA
nanostructures designed using an “RNA origami” strategy
should have potential to expand the variety of multidimensional
structures for the design and construction of novel RNA
In this study, we designed and prepared RNA origami
structures that were assembled from the single-stranded RNA
Prof. Dr. M. Endo, K. Hidaka, Prof. Dr. H. Sugiyama
Institute for Integrated Cell-Material Sciences (WPI-iCeMS), Kyoto
University, Yoshida-ushinomiyacho, Sakyo-ku, Kyoto 606-8501
Fax: (+81) 75-753-3670
E-mail: [email protected]; [email protected]
Y. Takeuchi, T. Emura, Prof. Dr. H. Sugiyama
Department of Chemistry, Graduate School of Science, Kyoto
University, Kitashirakawa-oiwakecho, Sakyo-ku, Kyoto 606-8502
Title(s), Initial(s), Surname(s) of Author(s) including Corresponding
Dr. M. Endo, Prof. Dr. H. Sugiyama
Japan Science and Technology Agency (JST),
Institution Chiyoda-ku, Tokyo 102-0075 (Japan)
work was supported by Core Research for Evolutional Science
and JSPS KAKENHI (Grant
24225005, 24310097, 24104002, 26620133). Financial
Institutionfrom The Mitsubishi Foundation and The Asahi Glass
Address 2 to ME are also acknowledged.
given via on
the end of
scaffold and staple RNA strands (Figure 1a). The RNA origami
for a 7-helix bundled planar structure (7HB-tile) was designed
with a geometry of 33 bp per three turns in the adjacent
crossover points, which corresponds to a helical pitch with 11
bp/turn. The RNA duplex forms an A-form structure with an 11
bp/turn helical pitch, which means that a geometrical design with
11 bp/turn should be structurally stable. For the design of a 6helix bundled tubular structure (6HB-tube), we used the
geometry of the usual DNA origami design.
Figure 1. Preparation of RNA origami. (a) The RNA scaffold was prepared by
in vitro transcription using a template dsDNA containing the T7 promoter using
T7 RNA polymerase. Staple RNA strands were prepared by in vitro
transcription from biotinylated dsDNAs. Subsequently, a 7-helix bundled (7HB)
tile and a 6-helix bundled (6HB) tube were assembled from purified RNA
scaffold and staple RNA strands. (b) Modified uridine triphosphate (UTP), 5biotinylated UTP and 5-aminoallyl UTP were used for the synthesis of modified
RNA transcripts for the preparation of the chemically modified RNA origami
First, an RNA transcript for the scaffold was obtained from a
double-stranded DNA (dsDNA) template by in vitro transcription
using T7 RNA polymerase. In the preparation of staple RNA
strands, dsDNA templates were obtained from a biotinylated T7
primer and template single-stranded DNAs that were specific for
the staple strands, using DNA polymerase (Klenow fragment).
Subsequently, the staple RNA strands were obtained from
biotinylated dsDNA templates using T7 RNA polymerase.
Biotinylated dsDNAs were removed by streptavidin–magnetic
beads and the solutions were subjected to ethanol precipitation
or gel filtration for the purification of the RNA staple strands.
RNA/DNA hybrid tiles were compared with those of the RNA
origami tiles (Table 1). In the case of the planar tiles, the axial
lengths of the RNA/DNA tiles (33.4 nm) were similar to those of
the RNA origami tiles (Table 1). Both the RNA tile and the
RNA/DNA hybrid tiles formed similar structures.
Figure 2. Complex formation of RNA origami structures. (a) Polyacrylamide
gel electrophoretic (4%) analysis of 7HB-tile assemblies with modified UTPs.
(b) PAGE analysis of 6HB-tube assemblies with modified UTPs.
To examine the RNA origami tile, we prepared the 7HB-tile
structure (Figure 1). The RNA template was mixed with a staple
RNA strand mixture (40 equivalents excess) in a solution
containing 20 mM Tris buffer (pH 7.6), 10 mM MgCl2 and 1 mM
EDTA. The mixture was annealed from 75 °C to 20 °C at a rate
of –0.5 °C/min. The assembled structures were purified by gel
filtration, and characterized by native polyacrylamide gel
electrophoresis and atomic force microscopy (AFM). In the
native polyacrylamide gel electrophoresis (PAGE) analysis, the
RNA assembly showed a clear band (Figure 2a). The AFM
images (Figures 3a and S1a) showed that RNA tile assemblies
formed rectangular structures. The formation of the 7HB-tile
structure was observed as a correct rectangular shape with
dimensions of 32.5 × 21.2 nm (Figure 3b). The yield obtained
from the AFM images was 58% (N = 439). The rise per base pair
for the A-form RNA duplex was 0.28 nm; thus, the observed
length of the axial direction was 33 nm, which was 12% longer
than expected length (28 nm). The difference in the sizes in the
axial direction may be attributed to the expansion of the A-form
structure in the constrained and packed nanostructure.
Next, a 6HB tubular structure was prepared from the RNA
scaffold and staple RNA strands using the same annealing
conditions (Figure 1c). The assembled structures were observed
by AFM and analysed by native PAGE. In the native PAGE
analysis, the assembled tube showed a clear band (Figure 2b).
The AFM images showed that the assemblies formed rod-like
structures that were 41.2 nm in length and 5.7 nm in height, in
which the height was twice that of the planar tiles on the 3aminopropyl-triethoxysilane-passivated mica surface (Figures 3c
and S2a). The yield of tube formation determined after gel
filtration was 44% (N = 81). Therefore, the structural stress
originating from the 10.5 bp/turn helical pitch in the RNA duplex
seemed to be relatively small for the formation of the RNA
To compare the RNA origami structures with the RNA/DNA
hybrid origami structures, RNA/DNA origami structures were
prepared using the purified single-stranded RNA template and
the DNA staple strands. RNA/DNA hybrid origami structures
were correctly formed under the same conditions used for RNA
origami formation (Figures S3a and S4a). The sizes of the
Figure 3. AFM images of RNA origami structures. (a) AFM images of 7HB-tile
assemblies. (b) Detailed images of the 7HB RNA origami tile. (c) AFM images
of the 6HB RNA origami tubular structure.
Table 1. Observed dimensions of the 7HB-tile and 6HB-tube RNA origami
structures and RNA/DNA hybrid structures.
length x width or height (nm)
RNA origami 7HB tile
32.5 ± 1.9 x 21.1 ± 0.9
RNA origami 6HB tube
41.2±2.8 x 5.7 ± 0.4
RNA/DNA origami 7HB tile
RNA/DNA origami 6HB tube
Mean ± S.D.
33.4 ± 1.5 x 22.5 ± 1.5
39.0 ± 1.1 x 4.0 ± 0.1
Height of the structure.
To expand the chemical modification of origami structures,
the modified RNA templates were used for RNA origami
formation. Native UTP was fully replaced by 5-biotinylated UTP
and 5-aminoallyl UTP for the preparation of chemically modified
RNA scaffolds. The RNA scaffolds containing modified uracil
and staple strands were annealed using the conditions
In the native PAGE analysis, the modified RNA assemblies
showed clear bands (Figure 2a). Both bands were shifted
compared with that of the unmodified RNA origami tile. The
hydrophobicity of biotin and the cationic property of the
aminoallyl group in the modified RNA scaffolds changed their
migration in the polyacrylamide gel. In the case of the 5biotinylated uracil modification, the hydrophobicity of biotin led to
a slower migration compared with the unmodified RNA origami
tile. In the case of the 5-aminoallyl uracil modification, the
positive charge of the primary amine neutralized the negative
charge of phosphates, resulting in a slightly slower migration.
These results showed that modification at the 5-position of uracil
changes the physical properties of the assembled RNA origami
structures. These assembled structures were observed by AFM
(Figures 4 and S3). The AFM images showed that RNA origami
tiles were also formed using RNA scaffolds that contained
modified uracil (Figure 4). The observed dimensions of the
structures that included 5-biotinylated uracil and 5-aminoallyl
uracil were 32.8 × 22.2 nm and 33.8 × 21.6 nm, respectively
(Table 2). The yields of origami tile formation using the RNA
templates containing 5-biotinylated uracil and 5-aminoallyl uracil
were 53% (N = 158) and 52% (N = 104), respectively. The
observed sizes were similar to those of the unmodified RNA
prepared using an RNA template with 5-biotinylated uracil. (D) 6HB-tube
assemblies prepared using an RNA template with 5-aminoallyl uracil. Inset
image size: 50 × 50 nm.
In addition, tubular structures were obtained from the RNA
scaffolds that contained 5-biotinylated uracil and 5-aminoallyl
uracil. Their formation was confirmed by gel electrophoresis
(Figure 2b), and their observed dimensions were 37.6 nm and
38.3 nm in length and 6.2 nm and 4.3 nm in height, respectively
(Figures 4c,d and Table 2). The heights of the modified tubes,
because of the modification, changed by 0.5 and –1.4 nm for 5aminoallyl uracil and 5-biotinylated uracil, respectively,
compared with that of the unmodified tube (5.7 nm). The yields
of origami tube formation from the RNA templates that contained
5-biotinylated uracil and 5-aminoallyl uracil were 46% (N = 125)
and 47% (N = 52), respectively.
Table 2. Observed dimensions of modified 7HB-tile and 6HB-tube RNA
origami structures with 5-biotinylated uracil and 5-aminoallyl or -containing
32.8 ± 2.2 ×
22.2 ± 1.1
37.6 ± 3.7 ×
6.2 ± 0.4
33.9 ± 1.2 ×
23.5 ± 1.7
37.6 ± 2.5 ×
3.8 ± 0.4
33.1 ± 1.6 ×
21.6 ± 0.8
38.3 ± 1.2 ×
4.3 ± 0.
33.1 ± 1.1 ×
22.5 ± 1.1
40.0 ± 2.5 ×
3.7 ± 0.1
Mean ± S.D. Dimension, length × width or height (nm).
Height of the
The modified RNA origami structures were also compared
with the RNA/DNA hybrid origami structures. The hybrid tiles
formed good assemblies, as assessed by gel electrophoresis,
whereas the hybrid tubes did not form well (Figures S3b and S5).
In the case of the tube design, we used the 10.5 bp/turn helical
pitch, which is not suitable for the formation of tubular structures
based on an RNA/DNA hybrid. These results indicate that the
RNA/DNA hybrid duplex is not as flexible as the RNA duplex.
In conclusion, we successfully prepared RNA origami
structures using RNA scaffold and designed staple RNA strands
which were simply prepared via in vitro transcription.
Furthermore, the physical properties of the assembled structures
were changed by modification of the RNA scaffolds. This
method can be applied for the introduction of various functional
molecules into RNA nanostructures via chemical modifications
that express specific functions.
origami (Table 2).
Figure 4. AFM images of 7HB-tile and 6HB-tube RNA origami using an RNA
template in which uracil was replaced fully by 5-biotinylated uracil and 5aminoallyl uracil. (a) 7HB-tile assemblies prepared using an RNA template
with 5-biotinylated uracil. (b) 7HB-tile assemblies prepared using an RNA
template with 5-aminoallyl uracil. (c) AFM images of 6HB-tube assemblies
Materials. Single-stranded M13mp18 DNA and streptavidin magnetic
beads were purchased from New England Biolabs (Ipswich, MA). The
staple strands and primers were purchased from Operon Biotechnology
(Tokyo, Japan). Modified oligonucleotides were purchased from Nippon
Bio Service (Saitama, Japan). PCR amplification was carried out using
GoTaq Green Master Mix (Promega). 5-biotinylated UTP (Bio-16-UTP)
and 5-(3-aminoallyl)-UTP were purchased from Ambion (Austin, TX).
The gel-filtration column and the Sephacryl S-300 were purchased from
Bio-Rad Laboratories, Inc. (Hercules, CA) and GE Healthcare
(Buckinghamshire, UK), respectively.
AFM imaging. AFM images were obtained using an AFM system (Nano
Live Vision, RIBM, Tsukuba, Japan) with a silicon nitride cantilever
(Olympus BL-AC10EGS). Samples (2 µL) were adsorbed onto an
aqueous 3-aminopropyltriethoxysilane (APTES, 0.1%) passivated mica
plate for 5 min at room temperature and then washed three times using
the same buffer solution. Scanning was performed in the same buffer
solution using a tapping mode.
Preparation of template dsDNA for RNA synthesis. The PCR
amplification of the template dsDNA was carried out from a plasmidcontaining EGFP coding region (717 nt) using Go Taq (Promega) with
two primers by following the manufacture’s protocol, and the product was
purified using a PCR purification kit (Qiagen).
Preparation of RNA template and RNA staples. A T7 promotercontaining template dsDNA was used for the transcription to prepare
RNA template. RNA synthesis was performed using 10 nM template
dsDNA, 40 mM Tris-HCl (pH 8.0), 5 mM DTT, 8 mM MgCl2, 2 mM
spermidine, 0.5 mM NTP, and 0.25 µM T7 RNA polymerase (Takara) at
42 oC for 1.5 h. In the cases of the preparation of modified RNA
templates, UTP was replaced to 5-aminoally UTP and 5-biotinylated UTP.
The transcribed RNA was treated with DNAase (Takara) and purified
using RNeasy Mini kit (Qiagen). The product was confirmed by gel
Preparation of RNA staple strands. A biotine-attached primer of T7
promoter top strand was annealed with bottom strand containing
complementary strand of the target RNA staple strand and T7 promoter
bottom strand. The DNA strands were incubated with Klenow fragment
with dNTP to prepare dsDNA. After the deactivation of Klenow fragment
by heating at 65 oC for 20 min, the prepared dsDNA templates were
incubated with T7 RNA polymerase using the same condition above. The
reaction mixtures were mixed together and the biontinylated dsDNA
templates were removed by streptavidin-magnetic beads twice. The RNA
mixture was purified by gel filtration and used without further purification.
Preparation of RNA origami. The RNA origami was designed by a
caDNAno software  using the geometry of 11.00 bp/turn for tile and
10.50 helical pitch for tube. The sequences of the staple strands are
listed in Table S1. For the tile formation, sample solution (40 µL)
containing 0.02 µM RNA template, 1 µM staple RNA strands (40 eq), 20
mM Tris-HCl (pH 7.6), 1 mM EDTA, and 10 mM MgCl2 was annealed
from 75 °C to 15 °C at a rate of –1.0 °C/min. For the tube formation,
sample solution (40 µL) containing 0.02 µM RNA template, 0.4 µM staple
RNA strands (40 eq), 20 mM Tris-HCl (pH 7.6), 1 mM EDTA, and 10 mM
MgCl2 was annealed from 65 °C to 15 °C at a rate of –0.1 °C/min. These
structures were purified using a gel filtration column (Sephacryl 300, GE
Helthcare). The purified RNA origami was analysed with a 4% native
polyacrylamide gel electrophoresis (4%) run at 4 oC in 1xTBE buffer with
5 mM MgCl2.
Preparation of RNA origami with modified UTP. For the preparation of
modified RNA templates, in vitro transcription was performed with ATP,
CTP, GTP, and 5-biotinylated UTP or 5-aminoallyl UTP. The purified
modified RNA templates and staple strands were assembled as
This work was supported by Core Research for Evolutional
Science and Technology (CREST) of JST and JSPS KAKENHI
(grant nos. 24310097, 24104002, 25253004, ). Financial
supports from The Mitsubishi Foundation and The Asahi Glass
Foundation to ME are also acknowledged.
Keywords: RNA • nanostructure • transcription• chemical
modification • AFM
 P. Guo, Nat. Nanotechnol. 2010, 5, 833-842.
 G. C. Shukla, F. Haque, Y. Tor, L. M. Wilhelmsson, J. J. Toulme, H.
Isambert, P. Guo, J. J. Rossi, S. A. Tenenbaum and B. A. Shapiro,
ACS Nano 2011, 5, 3405-3418.
 J. L. Vinkenborg, N. Karnowski and M. Famulok, Nat. Chem. Biol. 2011, 7,
 S. Chakraborty, S. Mehtab and Y. Krishnan, Acc Chem Res 2014, 47,
 A. Chworos, I. Severcan, A. Y. Koyfman, P. Weinkam, E. Oroudjev, H. G.
Hansma and L. Jaeger, Science 2004, 306, 2068-2072.
 K. A. Afonin, W. W. Grabow, F. M. Walker, E. Bindewald, M. A.
Dobrovolskaia, B. A. Shapiro and L. Jaeger, Nat. Protoc. 2011, 6, 20222034.
 W. W. Grabow, P. Zakrevsky, K. A. Afonin, A. Chworos, B. A. Shapiro and
L. Jaeger, Nano Lett. 2011, 11, 878-887.
 E. F. Khisamutdinov, D. L. Jasinski and P. Guo, ACS Nano 2014, 8, 47714781.
 W. W. Grabow and L. Jaeger, Acc. Chem. Res. 2014, 47, 1871−1880.
 P. W. Rothemund, Nature 2006, 440, 297-302.
 J. Fu, M. Liu, Y. Liu, N. W. Woodbury and H. Yan, J. Am. Chem. Soc.
2012, 134, 5516-5519.
 S. H. Ko, M. Su, C. Zhang, A. E. Ribbe, W. Jiang and C. Mao, Nat. Chem.
2010, 2, 1050-1055.
 M. Endo, S. Yamamoto, K. Tatsumi, T. Emura, K. Hidaka and H.
Sugiyama, Chem. Commun. 2013, 49, 2879-2881.
 P. Wang, S. H. Ko, C. Tian, C. Hao and C. Mao, Chem. Commun. 2013,
 S. M. Douglas, H. Dietz, T. Liedl, B. Hogberg, F. Graf and W. M. Shih,
Nature 2009, 459, 414-418.
 N. C. Horton and B. C. Finzel, J. Mol. Biol. 1996, 264, 521-533.
 S. M. Douglas, A. H. Marblestone, S. Teerapittayanon, A. Vazquez, G. M.
Church and W. M. Shih, Nucleic Acids Res. 2009, 37, 5001-5006.
Entry for the Table of Contents
RNA nanostructures were designed
and prepared using the DNA origami
strategy. Predesigned 7-helix bundled
RNA tile and 6-helix bundled RNA
tube nanostructures were obtained by
annealing of a single-stranded RNA
scaffold and staple RNA strands.
These nanostructures were easily
functionalized by introduction of the
chemical modification to the RNA
Masayuki Endo,* Yosuke Takeuchi,
Tomoko Emura, Kumi Hidaka, and
Page No. – Page No.
Preparation of Chemically Modified
RNA Origami Nanostructures